Pure organochlorides like polyvinyl chloride (PVC) do not absorb any light above 220 nm. The initiation of photo-oxidation is instead caused by various irregularities in the polymer chain, such as structural defects as well as hydroperoxides, carbonyl groups, and double bonds. 
Hydroperoxides formed during processing are the most important initiator to begin with, however their concentration decreases during photo-oxidation whereas carbonyl concentration increases, as such carbonyls may become the primary initiator over time.
Propagation steps involve the hydroperoxyl radical, which can abstract hydrogen from both hydrocarbon (-CH-) and organochloride (-CHCl-) sites in the polymer at comparable rates. Radicals formed at hydrocarbon sites rapidly convert to alkenes with loss of radical chlorine. This forms allylic hydrogens (shown in red) which are more susceptible to hydrogen abstraction leading to the formation of polyenes in zipper-like reactions.
When the polyenes contain at least eight conjugated double bonds they become coloured, leading to yellowing and eventual browning of the material. This is off-set slightly by longer polyenes being photobleached with atmospheric oxygen, however PVC does eventually discolour unless polymer stabilisers are present. Reactions at organochloride sites proceed via the usual hydroperoxyl and hydroperoxide before photolysis yields the α-chloro-alkoxyl radical. This species can undergo various reactions to give carbonyls, peroxide cross-links and beta scission products.